Journal Pre-proof Wear induced ripplocation during dry sliding wear of TiC-based composite Carl Magnus, Ali Mostaed, William M. Rainforth PII:
To appear in:
Received Date: 26 April 2019 Revised Date:
17 September 2019
Accepted Date: 8 November 2019
Please cite this article as: C. Magnus, A. Mostaed, W.M. Rainforth, Wear induced ripplocation during dry sliding wear of TiC-based composite, Wear (2019), doi: https://doi.org/10.1016/j.wear.2019.203121. This is a PDF file of an article that has undergone enhancements after acceptance, such as the addition of a cover page and metadata, and formatting for readability, but it is not yet the definitive version of record. This version will undergo additional copyediting, typesetting and review before it is published in its final form, but we are providing this version to give early visibility of the article. Please note that, during the production process, errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain. © 2019 Published by Elsevier B.V.
Wear induced ripplocation during dry sliding wear of TiC-based composite Carl Magnus1,2, Ali Mostaed1 and William M. Rainforth1 1
Department of Materials Science and Engineering, The University of Sheffield, Mappin Street, Sheffield S1 3JD, UK. 2
Anton Paar TriTec SA, Rue de la Gare 4, 2034 Peseux, Switzerland.
Abstract Monolithic TiC and TiC composite containing 30 and 50 mol.%SiC were consolidated and synthesized using spark plasma sintering (SPS) without sintering aids. The as-sintered bulk samples microstructural and dry sliding room-temperature tribological properties against Al2O3 were characterized using X-ray diffraction (XRD), scanning electron microscopy (SEM), transmission electron microscopy (TEM) and Raman analyses. The role of mismatch in coefficient of thermal expansion (CTE) between TiC and SiC as well as cubic to hexagonal SiC phase transformation on the evolution of residual stresses in the composite was also investigated. The friction and wear properties of the monolithic TiC were superior to that of the composite with frictional heating-induced tribo-oxidation playing a dominant role in the wear mechanism. The increase in friction and wear of the composite is attributed to wearinduced stress-relaxation of the previously trapped residual stresses in the composite leading to extensive ripplocation of the TiC grains and consequent SiC grain pull-outs. Herein, we report for the first time on the wear-induced mechanical exfoliation of carbon, its subsequent decomposition into graphite and eventual deformation by micromechanism involving nucleation and propagation of ripples. Keywords: Spark Plasma Sintering; High Temperature Ceramics; Dry Sliding Friction; Frictional Heating; Residual Stresses; Thermal Expansion; Ripplocations; Exfoliation
The brittleness and flaw sensitivity of TiC and SiC ceramics which has limited their use as structural material in monolithic state has led to the development of TiC-SiC particulate composite system with improved fracture toughness [1, 2]. Silicon carbide exists in two forms, the α (hexagonal) and β (cubic), with the hexagonal form exhibiting many prototypes . SiC possesses only three possible slip systems, as a result, dislocation motion is impeded and motion of dislocation occur only on a very limited scale , thus fracture toughness is much lower as compared to metals. Addition of TiC particles into a SiC matrix or SiC particles into a TiC matrix has been found to yield promising composite systems with
significantly improved strength and toughness [2, 4]. The increase in fracture toughness to about three or four times as large as that of monolithic states  has been associated predominantly with misfit of coefficient of thermal expansion (CTE) between the matrix and the second phase . Misfit in thermal expansion introduces significant radial stresses at the phase boundaries and hoop compressive stresses inside the matrix. These stresses promote toughening mechanisms such as crack deflection, crack branching and stress-induced microcracking . According to Wasche and Ajayi et al. [7, 8], the incorporation of particles of a second phase into monolithic ceramics can improve significantly their tribological behaviour, especially in unlubricated conditions. The resulting composite will enable the exploitation of the excellent wear properties of SiC whilst simultaneously benefitting from the high thermal expansion coefficient mismatch between TiC and SiC . Currently, a comprehensive practical understanding of the role of residual stresses due to misfit in coefficient of thermal expansion between the matrix and the particle on wear behaviour is lacking, even though it has been well established theoretically that internal residual stresses can influence the fracture and wear resistance of composites . The objective of this work is to fabricate monolithic TiC and TiC-SiC composite systems using spark plasma sintering (SPS) and investigate their dry sliding tribological properties. In addition, the role of mismatch in thermal expansion coefficient between TiC and SiC upon synthesis on the wear behaviour of the resulting TiC-SiC composite will be explored. 2.
Ceramic material fabrication and characterization
Commercially available silicon carbide powder (cubic structure (β-SiC), 99.8 % purity, 1µm Alfa Aesar) and titanium carbide powder (99.5 % purity, 2 µm Alfa Aesar) were mixed according to Table 1 and ball milled in isopropanol using a 1.0 mm diameter zirconia ball at room temperature for 24 hours. The milled powder was then sieved using a 200 mesh sieve and subsequently synthesized by the spark plasma sintering (SPS) powder metallurgy method. Details of the sample composition and synthesis are summarized in Table 1. Phase analysis of the SPSed polished unetched disc surfaces was carried out on a diffractometer (Bruker X/154 D2 Phaser, Germany) with Cu Kα radiation source using a step size of 0.02° and time per step 3 sec over a 2Ө range from 5° - 80°. The microstructural evolution of the pristine and worn samples as well as toughening mechanisms were investigated by Vickers indentation (DuraScan G5, emco TEST), scanning electron
microscopy (SEM) (FEI Inspect F50, The Netherlands) in conjuction with energy dispersive X-ray spectroscopy (EDS, Oxford Instrument X-Max / Aztec Microanalysis, UK) and transmission electron microscopy (TEM), (FEI Tecnai Spirit / JEOL 3100Z R005 aberration corrected high-resolution TEM). TEM samples were prepared using a focused ion beam, (FIB), (FEI Helios NanoLab G3 UC, FEI company, The Netherlands) by lifting out sections from the pristine and worn surface which were then further thinned down using FIB for TEM analyses. Raman analyses was carried out ex-situ on the pristine and worn surfaces by employing a Si-calibrated inVia Raman spectrometer (Renishaw plc, UK) with an Ar laser (λ = 514.5 nm, laser output power 20 mW) and a 50x objective lens (spot size of 2 µm). Optical microscopy was used to further analyse the alumina balls after each test to investigate any possible material removal, oxidation and/or transfer materials from the bulk sample. Table 1. Sample details and SPS sintering parameters Elemental powder
SPS sintering details
*Pre-press load; 641 kg, graphite die; 20 mm, heating rate; 100 °C/min sintering pressure; 50 MPa, and SPS unit (HP D 25 FCT Systeme, Germany).
Further details of the SPS synthesis and processing conditions are reported elsewhere . 2.2.
Unlubricated sliding wear tests were carried out using a ball on disk configuration (ball: Al2O3 (2 mm) and disk: monolithic TiC and TiC-SiC composite) in ambient conditions (25 °C and 38% RH) on a commercially available tribometer (TRB Anton Paar TriTec SA, Peseux, Switzerland). An Al2O3 ball was utilized as the counterface due to its relative inertness, as it would not be expected to react with the bulk sample and has been widely used in wear testing of TiC-based composites, and therefore the current results can better be compared to those in the literature. Tribological tests were conducted using a normal load of 2 N and rotational speed at 200 rpm which corresponds to a total sliding distance of 445 km for an hour. Schematic of the rotary configuration employed using the pin-on-disk tribometer is shown in Figure 1. The frictional force and the normal load were continuously monitored
by the load cell and the friction coefficient (CoF) was recorded in real time during the test. The specific wear rate was estimated by using Eq. (1) upon measuring the length and width of the wear track to determine the worn volume. ⁄
Where K = specific wear rate (mm3/Nm), V = wear volume (mm3), FN = load (N), and Sd = sliding distance (m), respectively.
Fig. 1. Schematic of an Anton Paar tribometer employed for friction and wear test.
Results and Discussion
3.1. Phase analysis, densification, hardness and microstructure The XRD patterns of the synthesized TiC-based ceramic compositions are presented in Figure 2. As seen in the diffraction patterns, TiC and SiC phases were the only crystalline phases present indicating no solid solution reaction between the TiC and SiC phases. Also, as TiC and β-SiC are cubic in nature, their phases were somewhat indistinguishable owing to similar lattice parameters. However, some distinct peaks of α-SiC were detected due to possible phase transformation from β → α – (SiC) at sintering temperature above 1800 °C.
Fig. 2. X-ray diffraction patterns of the synthesized polished disc samples.
SPS produced near-fully dense bulk specimens for both the monolithic and composite compositions. The resulting SPS sintered compacts attained 98 % density for monolithic TiC, 99 % for TiC-50 mol.%SiC, and only 92 % for TiC-30 mol.%SiC, upon taking into account the theoretical densities of TiC (4.92 g/cm3) and SiC (3.21g/cm3), respectively. Vickers hardness measurement revealed that the hardness of the composite TiC-50 mol.%SiC was slightly higher than that of the monolithic TiC. For the measured values, the composite TiC50 mol.%SiC exhibit the highest hardness ~ 3180 HV followed by the monolithic TiC ~ 3000 HV. The composite TiC-30 mol.%SiC exhibited somewhat the lowest hardness ~ 2750 HV which is quite surprising. According to the volumetric rule of mixtures, the hardness values of the composites are expected to be way higher than recorded . However, due to thermal expansion mismatch between SiC and TiC, the work of indentation may have been reduced due to the distribution of residual stresses in the composite . The microstructure (Figures 3 and 4) of the TiC-SiC composite consist of two distinct phases of elongated particles of SiC (dark phase) homogeneously distributed in the TiC matrix (bright phase) as identified by EDS analysis (Figure 5). The presence of only two major phases is in agreement with the lack of solid solutions found in the SiC-TiC pseudo-binary
system . It is noteworthy to mention that a possible reason for SiC grain elongation is linked to possible β-(SiC)
α-(SiC) phase transformation taking place during synthesis
as explained elsewhere . In comparison to the grain size of the monolithic TiC, the grain size of TiC in the TiC-SiC composite appears smaller. This can be attributed solely to the matrix grain-boundary pinning effect by the SiC particles during the sintering which inhibits the exaggerated TiC grain growth .
Fig. 3. Optical micrographs of the polished discs: (a) monolithic TiC and (b) TiC-50 mol.% SiC
Fig. 4. SEM micrographs of the SPSed polished unetched surfaces of the discs: (a) monolithic TiC and (b) TiC-50 mol.% SiC composite. Note: white contrasts are artefacts from colloidal silica.
Fig. 5. EDS map analysis of the polished surface of the TiC-50 mol.%SiC showing the elemental distribution.
3.1.1. TEM of pristine surface of composite Figure 6 shows TEM micrographs taken from the pristine surface of the TiC-50 mol.%SiC composite system. The TiC grain is essentially defect-free whilst profuse stacking fault can be seen in the SiC grain (1) (Fig. 6(a)). Higher magnifications of the SiC grain (1) further highlights the extent of the planar defect (stacking faults) which has been linked to the low stacking fault of energy in SiC (Fig. 6(b)). Evidence of partial dislocation (arrow in Fig.6(b)) can also be seen and represents the mechanism by which the growth of α-SiC nucleates (i.e.,
partial dislocation motion). This indicates that partial β→α phase transformation of SiC may have taken place during the SPS in consistent with the XRD analysis. To further verify the possible β→α phase transformation due to SPS above 1800 °C, TEM studies were done near the ˂110˃β zone axis to reveal reciprocal lattice rows from which both the β and α patterns can be easily identified (i.e., extra spots are introduced into the β diffraction pattern due to the α polytype) as well as enabling the simultaneous visualization of the β and (0001)α planes edge-on. Lattice fringe image obtained from a partially transformed plate-like SiC grain (2) is shown in Figure 6(c-f).
Fig. 6. (a) TEM bright-field image taken from the pristine surface of TiC-50 mol.% SiC composite, (b) higher magnification bright-field image taken from grain (1), (c-d) bright-field and dark-field lattice fringe image of β/α interface region in SiC grain (2) which has been partially transformed with an array of β twins evident at the centre, (e) SAED patterns showing extra spot due to twins and (f) HRTEM image in the  zone axis evidencing twins and stacking faults.
Figure 7 shows the characteristic evolution of the coefficient of friction with sliding time. For the TiC/Al2O3 couple subjected to sliding wear, the coefficient of friction was relatively stable throughout the entire test duration. This stable behaviour can be somewhat attributed to the formation of a triboreaction layer that appears stable as a function of time. On the other hand, the coefficients of friction of the TiC-SiC/Al2O3 tribocouples appear to be very unstable with repeated fluctuations. The reason for this might be due to instability of the triboreaction layer formed, or because the tribo-reaction layer formed is repeatedly worn off upon formation. The steady state CoF mean value against Al2O3 was (0.19 ± 0.01) for TiC, (0.35 ± 0.02) for TiC-30 mol.%SiC, and (0.39 ± 0.01) for TiC-50 mol.%SiC composite, respectively.
Fig. 7. Evolution of the friction coefficient with sliding time for rotational dry sliding contacts TiC/Al2O3 and TiC-SiC/Al2O3 composites at room temperature.
The specific wear rate of TiC and the TiC-SiC composites against Al2O3 ball is plotted in Figure 8. In general, the corresponding wear measurements reveal a correlated behaviour that is consistent with the friction curve. The specific wear rate is lower for the TiC/Al2O3 tribocouple than for the TiC-SiC/Al2O3 composites, indicating a major role of tribo-oxidation product in the wear mechanism. The TiC-SiC composite exhibited approximately 3 times more wear against Al2O3 as compared to monolithic TiC. It is believed that TiC reinforced with large amount of SiC would intrinsically exhibit higher fracture toughness that would lead to reduced mechanical fracture or grain pull-out during sliding contact . However, the higher specific wear rate of the TiC-SiC composites as compared to monolithic TiC would imply that toughening-induced fracture toughness was inactive or possibly inefficient during the shear sliding contact. Almost comparable data on the friction and wear on a range of SiC-TiC composite system sliding against Al2O3 is presented elsewhere  albeit slight differences in testing parameters.
Fig. 8. Plot of the specific wear rate and friction coefficient as a function of composition.
In the following and owing to the scope of this work, microstructural analyses will be focused essentially on the TiC-50 mol.%SiC. 3.4.
Since no observable Raman active vibration modes are present in stoichiometric TiC [9, 19], Raman spectra were collected from the β-SiC starting powder and bulk SPSed TiC-SiC composite as shown in Figure 9. The spectrum of the bulk TiC-SiC composite revealed characteristic peaks of the vibration mode of α-SiC indicating a phase transformation from cubic (β) → hexagonal (α) during SPS, especially with the presence of α-SiC distinctive peak at 973 cm-1 consistent with results obtained elsewhere [9, 20]. The implication of such transformation is evident as observed in the microstructural evolution of the synthesized TiCSiC composite in which equiaxed β-SiC grains transforms to plate-like α-SiC grains.
Fig. 9. Raman spectra collected from the β-SiC powder and the resulting SPSed bulk TiC-50 mol.%SiC composite pristine surface.
Raman analyses of the wear tracks of the TiC/Al2O3 and TiC-SiC/Al2O3 tribocouples are presented in Figures 10 and 11. In both cases, the acquired Raman peaks corresponded to vibrational modes of titanium oxide (typically rutile) and graphitic carbon upon comparing to literature data [21-23]. The formation of rutile would imply that anatase TiO2, whose formation temperature is around ~ 500 °C, has been transformed into rutile as the temperature of the sliding surface increases due to frictional heating in accordance with ; Anatase TiO
The Raman spectrum obtained from the composite shows lower intensity of TiO2 peaks above the background in comparison to monolithic TiC. This could be attributed to the fact that the incorporation of SiC particles into the TiC matrix has reduced the amount of TiO2 that can be formed due to frictional heating during dry sliding. On the other hand, the graphitic layer formed in the wear track of the composite appear to be much more intense compared to the background than the graphitic carbon peaks in the Raman spectrum of TiC/Al2O3 wear track. The reason for this is not fully understood but it is conceivable that SiC is responsible for the increased graphitization of the TiC-SiC/Al2O3 tribocouple sliding interface.
Fig. 10. Raman spectra obtained inside in the wear track of the TiC/Al2O3 tribocouple. Inset is an optical micrograph indicating the location on the wear track.
Fig. 11. Raman spectra obtained inside in the wear track of the TiC-50 mol.%SiC/Al2O3 tribocouple. Inset is an optical micrograph indicating the location on the wear track.
Post-mortem SEM analysis of wear track
Post mortem SEM and EDS assessments of the sliding interface of the TiC/Al2O3 tribocouple are presented in Figures 12 and 13. The wear scar of the TiC/Al2O3 sliding surface appears to be moderately damaged with minimal grain fracture and subsequent pulverization evident. Sharp wear grooves can also be seen along the wear track. Tribofilms appear not to be visible inside the wear track even though Raman analysis revealed the evolution of tribo-oxidation products. This may be due to the fact that they have been worn off and/or incorporated and mixed with the wear debris. Nonetheless, EDX analysis of the fractured surface (Fig. 12(b)) presented in Figure 13 is quite consistent with Raman analysis in finding oxides on the surface.
Fig. 12. Post-mortem topographical (SE-BSE) SEM micrographs of the sliding surface of TiC/Al2O3 tribocouple.
Fig. 13. EDX elemental map analysis taken at the sliding surface of TiC/Al2O3 tribocouple.
The sliding surface of the TiC-SiC/Al2O3 tribocouple on the other hand is presented in Figure 14. Severe wear grooves (Fig.14(a)) running parallel across the wear track and fracture of the grains (Fig.14(c-d)) are observed. In addition, tribofilms (Fig.14(b)) as well as extensive rippling of the TiC grains (Fig.14(e-f)) are evident in the wear track. The reason for the rippled TiC grains is not fully clear, however, it might be linked to the thermal expansion mismatch between TiC and SiC. In general the observed grain damage is surprising given the high content of easy-shearing graphitic material observed in the wear track of TiC-SiC/Al2O3 tribocouples using Raman analysis. Nonetheless, the observed microstructural damage seems to explain the higher coefficient of friction measured for the TiC-SiC/Al2O3 tribocouples as compared to monolithic TiC.
Fig. 14. Post-mortem topographical SEM micrographs of the contacting surface of the TiC-50 mol.% SiC/Al2O3 tribocouple. Note (a and b) are SE-images whilst (b-c) and (e-f) are SE-images and their corresponding backscattered (BSE) images.
Figure 15 shows the comparative SEM-EDS elemental map analyses of an area inside the wear track of the TiC-50 mol.%SiC composite system. Preferential oxygen concentration around the TiC region can be observed which suggests possible TiO2 oxide formation in consistent with the Raman analysis. However, it is difficult using EDS analysis to distinguish between the intrinsic carbon content from the bulk sample composition and the graphitic layer formed due to the tribochemical reaction.
Fig. 15. EDS elemental map analysis taken from the worn surface of the TiC-50 mol.%SiC composite.
To further understand the wear mechanism, the surface of the alumina balls were analysed after each test. Analysis of the alumina ball after dry sliding against monolithic TiC (Fig. 16) showed evidence of some transfer film from the bulk material unto the ball surface as well as minor wear of the ball. The alumina ball surface after dry sliding against TiC-50 mol.%SiC (Fig. 17) showed that some wear debris was transferred to the ball surface from the bulk material. In addition, the ball surface appeared relatively rough and covered with compacted oxidized wear debris and/or smeared tribofilm. Wear grooves parallel to the sliding direction were also visible on the surface of the ball. It appears that debris accumulation on the surface of the ball grows as a function of time and ultimately enough debris is entrapped between the ball and the disc which then acts as a load bearing third-body. As a result, there will be an increase in contact force due to point contacts with particles, thus bringing about fluctuations in friction behaviour and increase in friction coefficient as observed in the composites.
Fig. 16. Optical images of the alumina ball surface after dry sliding against monolithic TiC.
Fig. 17. Optical images of the alumina ball surface after dry sliding against TiC-50 mol.%SiC.
As seen in Figure 4, the presence of SiC particles in the TiC matrix inhibited the exaggerated grain growth of the TiC grains, and as a consequence, toughening mechanisms will be initiated according to [1, 25, 26]. Furthermore, in addition to the SiC pinning toughening effect, the mismatch in coefficient of thermal expansion between TiC and SiC will introduce an additional toughening mechanism [1, 27]. This is because the thermal expansion coefficient of TiC is larger than that of SiC (αSiC ≈ 5.3 x 10-6 °C-1 and αTiC ≈ 7.4 x 10-6 °C-1, respectively ) and as a consequence hydrostatic compressive stress will be generated within the SiC grains . At the same time, radial compressive stress and tangential tensile stress will be generated in the TiC matrix around the SiC particles [1, 26]. Thus, if SiC is located on a crack extension plane, the crack will preferentially first reach the boundary of the TiC and SiC grains, as the surface energy of the SiC grains is larger than the interface
surface fracture energy of the TiC/SiC interface . As a result the crack will bypass the TiC matrix and SiC particle and instead propagate along the TiC/SiC interface . However, occasionally, the crack will propagate through the particle if they possess irregular shape and size [26, 29]. Figure 18 is a typical SEM micrograph of the trajectories of indentation cracks in the TiC-50 mol.%SiC composite. Energy absorbing toughening mechanisms such as crack deflection, crack branching and crack bridging are evident.
Fig. 18. Toughening mechanism in TiC-SiC composite with crack propagating preferentially along the grain boundary and occasionally deviating into the TiC and SiC grains.
Thermal expansion mismatch and residual stress
It has been well established that particulate composites generally contain inherent residual stresses by virtue of the mismatch in thermal expansion between the matrix and the particles, which is likely to initiate spontaneous microcracking when the second phase particle size attains a critical value [30, 31]. SEM investigation of the as-synthesized SPSed composite showed no evidence of neither microcracking nor fracture which would imply that the second phase SiC particle size distribution is below the critical size where spontaneous microcracking will initiate . The absence of cracks also implies that stresses due to thermal expansion mismatch have not been relieved, thus strain due to the thermal cycling
during the synthesis is retained in the composite (i.e., stress relaxation has not occurred). SEM observation of the composite wear track, in contrast to the worn surface of the monolithic TiC, revealed evolution of stress relaxation upon dry sliding contact. The TiC grains in the TiC-SiC composite is observed to have undergone severe rippling preferentially (Fig. 19) with no rippling behaviour observed in the SiC grains. This strongly suggests that stress due to thermal mismatch has been relieved (i.e., stress-relaxation) during the wear process. According to Luan et al. , residual stress trapped in composites could be relaxed significantly when there is a subsequent mechanical loading that causes superposition of the applied stress and residual stress via stress-induced microcracking [30, 33]. Such consequent stress-induced microcracking is expected to shield a propagating crack by the release of residual stress around the applied load [34, 35] i.e., toughening. However, the beneficial compressive stresses appear to have been worn off during the wear process, rendering toughening mechanisms such thermal residual toughening and microcracking inactive or inefficient against future loading, as only detrimental tensile stresses are left behind in the matrix that promotes severe rippling and consequent microcracking of the surrounding grains.
Fig. 19. SEM micrographs of the worn surface of the TiC-50 mol.%SiC composite showing evidence of extensive TiC grain ripplocation upon stress-relaxation. Note: (b) is a higher magnification of a section in (a).
In order to further provide detailed overview of the buckled section, 3D data were obtained from SEM images of the rippled section by employing 3D –image analytic software (MountainsMap® SEM Topo, Digital Surf, France) to reconstruct the backscatter SEM image. From the SEM 3D reconstruction (Fig. 20), extensive SiC grain pull-outs and fracture can be seen around the rippled TiC grains. It appears that the SiC grains are pulled out due to TiC grain ripple formation nearby and subsequently pulverized due to the contact load. Whilst the TiC grains on the other hand undergo micro and macro-fracture due to the residual stress relaxation.
Fig. 20. 3D-SEM reconstruction done on the rippled TiC grains from the wear track of the TiC-50 mol.%SiC composite.
It is noteworthy to mention that similar TiC grain ripplocation was observed in the TiC-30 mol.%SiC composite system. This strengthens the fact the observed TiC grain ripplocation is not a one-off event in the TiC-50 mol.% SiC composite system. 3.8.
TEM analyses of the rippled region
Focused ion beam (FIB) was used to prepare a cross-sectional TEM specimen containing the rippled TiC region (region of interest) inside the wear track. Figure 21 shows the lift-out process for preparing the TEM specimen.
Fig. 21. Ion-induced secondary electron micrographs of FIB sample preparation, showing location where the ripples were extracted inside the wear track and the final electron transparent TEM sample.
Figure 22 shows TEM images obtained from the rippled TiC grains. Upon careful observation from TEM images (e.g. Fig. 22) and EDS chemical maps (not shown here), a systematic mechanical exfoliation of carbon from the TiC grain was observed. According to the HRTEM image and its corresponding selected area electron diffraction (SAED) pattern obtained from the TiC-graphite interface (position marked by a yellow rectangle in Fig. 22(a)), the rippled graphite layers formed on the TiC grain where the graphite %001( are almost parallel to the TiC %100(. The ripples appear to be propagating along the %001(
graphite plane which is manifested on the surface of the TiC grains along the %100( plane. This highlights the crystallographic nature of this micromechanism.
Fig. 22. (a) Bright-field TEM micrograph obtained from the rippled region inside the composite wear track. Here, graphite layers are marked by “G”. (b) HRTEM image obtained from the TiC-graphite interface marked by a yellow rectangle in (a).
The observed ripplocations in the TiC grains are consistent with a new deformation mechanism termed bulk ripplocation (BR) as reported in 2D materials . Recently, layered solids such as graphite, MAX phases, MoS2 and mica have been reported to deform via a micromechanism involving the nucleation and propagation of ripplocations [36-39]. According to Kushima et al., ripplocation implies surface ripples and crystallographic dislocations and are essentially different to dislocations as such that they possess no Burgers vector or polarity [36, 37]. The formation of ripplocation is essentially associated to an atomic scale buckling which is not restricted to surfaces or near surfaces and can effectively occur in bulk in what was termed bulk ripplocations (BRs) . 3.9.
Mechanism of ripplocation formation
Superimposition of the shear stresses from the contact sliding load on the inherent tensile residual stresses around the TiC grains will lead to possible weakening of the Ti-C bond , thus the systematic mechanical exfoliation of carbon unto the surface of the TiC grains. The exfoliated carbon then decomposes into graphite due to frictional heating and subsequently deforms via a micromechanism involving the nucleation and propagation of ripplocation as
result of the repeated sliding contact. More work needs to be done to fully understand mechanisms leading to the exfoliation of carbon. 4.
Upon microstructural and chemical characterization of the worn surfaces of the bulk samples, the underlying wear mechanisms are elucidated as follows: 4.1.
Tribo-oxidation appears to be an operative wear mechanism according to the Raman analyses. The dry sliding nature of the tribological test seems to have generated enough frictional heating due to asperity temperature flashes to trigger selective oxidation of the TiC in both ceramic compositions (i.e., monolithic TiC and TiC-SiC composite). The tribooxidatively formed TiO2 alongside the graphitic layer acts as solid lubricant shielding the interface to prevent direct contact of the tribocouples. In the case of monolithic TiC, ‘oxidation-scrape-reoxidation’ appears to be taking place very rapidly such that limited contact is made between the tribocouples, thus the limited surface damage observed at the sliding surface of the TiC/Al2O3 tribocouple. For the composite, it seems that the oxidatively formed TiO2 has a lower fraction as compared to monolithic TiC simply due to the lower volume fraction of TiC in the composition. Since silicon has higher oxidation resistance than titanium, this explains the absence of silicon oxide in the Raman analysis of the composite wear track. The limited TiO2 formation will mean that repeated direct contact between the counterparts occurs faster, consistent with the instability seen in the friction plot of the TiCSiC/Al2O3 tribocouples. 4.2.
Abrasive wear was also an operational wear mechanism, this manifest by the evolution of horizontal grooves in the post-mortem sliding surfaces of both the monolithic and composite samples. The wear grooves tends to be more pronounced in the composite sample as compared to the monolithic TiC due to limited TiO2 tribofilms formed at the sliding surface causing extended contact between the tribocouples. The origin of the wear grooves as observed also on the surface of the ball may due to the fractured grains from the bulk material which detrimentally constitute an abrasive third-body. Fragments from the Al2O3 ball were
however not found in the wear track possibly due to its very low content or the area mapped by EDS and further probed by Raman did not contain the transfer material. 4.3.
Stress-relaxation induced wear mechanism
The simultaneous influence of the contact shear stress superimposed on the residual stress initiates the relief of the residual stresses previously trapped in the composite after sintering during the wear test. The relief of the residual stresses led to the weakening of the interface (grain boundary) strength that causes grain pull-outs and microcrack formation. The weakening of the interface enables easy pull-out of especially the SiC grains which is then subsequently fractured to constitute an abrasive third-body. This imply that the area in which beneficial compressive stresses prevail decreases, making toughening mechanism(s) less significant as wear progresses. As a result, detrimental tensile residual stress in the TiC grains will result in the ripplocation of the TiC grains due to the additional shear stresses imposed by the normal load during the sliding contact. The combination of SiC grain pull-outs due to stress relaxation and TiC grain ripplocation led to the increased friction coefficient and specific wear rate of the composite system. 5.
Monolithic TiC and TiC-SiC composite were successfully synthesized without sintering aids using SPS. The microstructure and tribological properties of the as-sintered samples were studied, and the following conclusions can be drawn: (1) Mismatch in thermal expansion between TiC and SiC as well as β→α SiC phase transformation led to high residual stresses in the composite system. (2) Tribofilms formation due to frictional heating induced tribo-oxidation acts as a protective layer at the disk/ball surface during sliding and reduces friction and wear of the counterparts. (3) Friction and wear behaviour of the monolithic TiC sample were superior to that of the composite albeit possessing better fracture toughness for the test condition. This is attributed to the incipient stress-relaxation and subsequent SiC grain pull-outs due to the shear stresses imposed upon sliding contact, thus generating abrasive third-body. (4) Mechanical exfoliation of carbon and its subsequent transformation into graphite due to frictional heating led to the deformation of the TiC grains via the nucleation of ripplocations.
Future exhaustive characterization will be needed to fully understand the combination of factors leading to the exfoliation of carbon from TiC as this is not fully understood at this time.
References 1. 2. 3. 4. 5.
6. 7. 8. 9.
12. 13. 14. 15.
16. 17. 18.
Wei, G.C. and P.F. Becher, Improvements in Mechanical Properties in SiC by the Addition of TiC Particles. Journal of the American Ceramic Society, 1984. 67(8): p. 571-574. Jiang, D.L., et al., Studies on the strengthening of silicon carbide-based multiphase ceramics I: The SiC-TiC system. Materials Science and Engineering: A, 1989. 109: p. 401-406. Stevens, R., Dislocation movement and slip systems in β-SiC. Journal of Materials Science, 1970. 5(6): p. 474-477. Chen, J., W. Li, and W. Jiang, Characterization of sintered TiC–SiC composites. Ceramics International, 2009. 35(8): p. 3125-3129. Kawai, C., K. Suzuki, and K. Tanaka, Fracture Toughness of TiC-SiC Composites Fabricated by CVD and the Mechanism of Toughening. Journal of the Ceramic Society of Japan, 1992. 100(1162): p. 835-840. Ralf Riedel, I.-W.C., Ceramics Science and Technology : Materials and Properties. Vol. Volume 2. 2010: Weinheim : Wiley-VCH. Wäsche, R., et al., Oscillating sliding wear behaviour of SiC, TiC, TiB2, 59SiC–41TiB2 and 52SiC–24TiC–24TiB2 materials up to 750°C in air. Tribotest, 2006. 12(2): p. 99-111. Ajayi, O.O., et al., Sliding Wear of Silicon Carbide—Titanium Boride Ceramic‐Matrix Composite. Journal of the American Ceramic Society, 1993. 76(2): p. 511-517. H., L.J., et al., Microstructure, Phase and Thermoelastic Properties of Laminated Liquid‐ Phase‐Sintered Silicon Carbide–Titanium Carbide Ceramic Composites. Journal of the American Ceramic Society, 2007. 90(7): p. 2189-2195. Gille, G. and K. Wetzig, Investigations on mechanical behaviour of brittle wear-resistant coatings I. Experimental results. Thin Solid Films, 1983. 110(1): p. 37-54. Magnus, C., T. Kwamman, and W.M. Rainforth, Dry sliding friction and wear behaviour of TiC-based ceramics and consequent effect of the evolution of grain buckling on wear mechanism. Wear, 2019. 422-423: p. 54-67. Srivatsan, T.S., et al., Influence of TiB2 content on microstructure and hardness of TiB2–B4C composite. Powder Technology, 2005. 159(3): p. 161-167. King, D.S., W.G. Fahrenholtz, and G.E. Hilmas, Silicon carbide–titanium diboride ceramic composites. Journal of the European Ceramic Society, 2013. 33(15): p. 2943-2951. Sowmya, A. and C.A. H., Synthesis of Titanium Silicon Carbide. Journal of the American Ceramic Society, 1995. 78(3): p. 667-672. Kim, Y.W., et al., Effect of Initial α‐Phase Content on Microstructure and Mechanical Properties of Sintered Silicon Carbide. Journal of the American Ceramic Society, 1998. 81(12): p. 3136-3140. H. McMurtry, C., et al., Microstructure and Material Properties of SiC-TiB2 Particulate Composite. Vol. 66. 1987. 325-329. Woydt, M., A. Skopp, and K.H. Habig, Dry friction and wear of self-mated sliding couples of SiC-TiC and Si3N4-TiN. Wear, 1991. 148(2): p. 377-394. Wäsche, R. and D. Klaffke, In situ formation of tribologically effective oxide interfaces in SiC‐based ceramics during dry oscillating sliding. Tribology Letters, 1998. 5(2): p. 173.
19. 20. 21. 22. 23. 24.
27. 28. 29. 30. 31. 32.
33. 34. 35. 36. 37. 38. 39. 40.
Brüesch, P., Phonons: theory and experiments. 2, Experiments and interpretation of experimental results. 1986, London: Springer-Verlag. Huong, P.V., Structural studies of diamond films and ultrahard materials by Raman and micro-Raman spectroscopies. Diamond and Related Materials, 1991. 1(1): p. 33-41. Klein, M.V., J.A. Holy, and W.S. Williams, Raman scattering induced by carbon vacancies in TiCx. Physical Review B, 1978. 17(4): p. 1546-1556. Balachandran, U. and N.G. Eror, Raman spectra of titanium dioxide. Journal of Solid State Chemistry, 1982. 42(3): p. 276-282. Tuinstra, F. and J.L. Koenig, Raman Spectrum of Graphite. The Journal of Chemical Physics, 1970. 53(3): p. 1126-1130. Pang, W.K., et al., 12 - Oxidation characteristics of Ti3AlC2, Ti3SiC2 and Ti2AlC, in Advances in Science and Technology of Mn+1AXn Phases. 2012, Woodhead Publishing. p. 289-322. Kim, Y.-W., S.-G. Lee, and Y.-I. Lee, Pressureless Sintering of SiC–TiC Composites with Improved Fracture Toughness. Vol. 35. 2000. 5569-5574. Ahmoye, D., Pressureless Sintering and Mechanical Properties of SiCComposites with in-situ Converted TiO2 to TiC, in Department of Mechanical and Materials Engineering. 2010, Queen’s University Kingston, Ontario, Canada. Endo, H., M. Ueki, and H. Kubo, Microstructure and mechanical properties of hot-pressed SiC-TiC composites. Journal of Materials Science, 1991. 26(14): p. 3769-3774. Kornaus, K., et al., Mechanical properties of hot-pressed SiC-TiC composites. Vol. 11. 2017. 329-336. Qin, C., et al., Microstructure Characterization and Mechanical Properties of TiSi2-SiCTi3SiC2 Composites Prepared by Spark Plasma Sintering. Vol. 47. 2006. 845-848. Gu, W.H. and K.T. Faber, Tensile behavior of microcracking SiC-TiB‐ composites. Journal of the American Ceramic Society, 1995. 78(6): p. 1507-1512. Magley, D., R. Winholtz, and K. Faber, Residual Stresses in a Two-Phase Microcracking Ceramic. J. Am. Ceram. Soc, 1990. 73(6): p. 1641-1644. Luan, W., C. Jiang, and V. Ji, Residual Stress Relaxation in Shot Peened Surface Layer on TiB2/Al Composite under Applied Loading. MATERIALS TRANSACTIONS, 2009. 50(1): p. 158-160. J., G.D., Stress‐Induced Microcracking at Second‐Phase Inclusions. Journal of the American Ceramic Society, 1981. 64(3): p. 138-141. Evans, A.G. and Y. Fu, Some effects of microcracks on the mechanical properties of brittle solids—II. Microcrack toughening. Acta Metallurgica, 1985. 33(8): p. 1525-1531. Evans, A.G. and K.T. Faber, Toughening of Ceramics by Circumferential Microcracking. Journal of the American Ceramic Society, 1981. 64(7): p. 394-398. Kushima, A., et al., Ripplocations in van der Waals Layers. Nano Letters, 2015. 15(2): p. 1302-1308. Gruber, J., et al., Evidence for Bulk Ripplocations in Layered Solids. Scientific Reports, 2016. 6: p. 33451. Barsoum, M.W., et al., Ripplocations: A universal deformation mechanism in layered solids. Physical Review Materials, 2019. 3(1): p. 013602. Griggs, J., et al., Spherical nanoindentation, modeling and transmission electron microscopy evidence for ripplocations in Ti3SiC2. Acta Materialia, 2017. 131: p. 141-155. Bartlett, A., A.G. Evans, and M. Rühle, Residual stress cracking of metal/ceramic bonds. Acta Metallurgica et Materialia, 1991. 39(7): p. 1579-1585.
HIGHLIGHTS: • • • • •
Spark plasma sintering (SPS) was used to synthesize fully dense monolithic TiC and TiC-SiC ceramic composite without sintering aids. Misfit of coefficient of thermal expansion (CTE) between TiC and SiC induce residual compressive and tensile stresses in the composite system. Incorporation of SiC particles into TiC matrix led to improved fracture toughness via crack bridging, crack branching, and crack deflection energy absorbing mechanisms. Oxide film formation is dependent on the phase fraction of TiC during dry sliding friction. Thermal expansion misfit induced grain ripplocations is a dominant wear mechanism in the composite system.
Statements for Conflicts of Interest
We the authors of this work hereby declare that there is no conflict of interest related to this work and this paper is an independent research carried out in our group at the department of engineering materials, University of Sheffield.